On the Lamellar Compounds CuBiP2Se6, AgBiP2Se6 and AgBiP2S6. Antiferroelectric Phase Transitions Due to Cooperative Cu+ and Bi3+ Ion Motion
Matthew A. Gave; Daniel Bilc; S. D. Mahanti; Jean D. Breshears; Mercouri G. Kanatzidis; Inorganic Chemistry 44 (2005) 5293–5303; doi:10.1021/ic050357+

data_4327330
_publ_section_title
;
 On the Lamellar Compounds CuBiP2Se6, AgBiP2Se6 and AgBiP2S6.
 Antiferroelectric Phase Transitions Due to Cooperative Cu+ and Bi3+ Ion
 Motion
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5293
_journal_page_last               5303
_journal_paper_doi               10.1021/ic050357+
_journal_volume                  44
_journal_year                    2005
_chemical_formula_sum            'Bi Cu P2 Se6'
_chemical_formula_weight         808.22
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           163
_symmetry_cell_setting           trigonal
_symmetry_space_group_name_Hall  '-P 3 2c'
_symmetry_space_group_name_H-M   'P -3 1 c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   6.5410(9)
_cell_length_b                   6.5410(9)
_cell_length_c                   13.263(3)
_cell_measurement_temperature    293(2)
_cell_volume                     491.43(15)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0577
_diffrn_reflns_av_sigmaI/netI    0.0328
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            1678
_diffrn_reflns_theta_full        22.51
_diffrn_reflns_theta_max         22.51
_diffrn_reflns_theta_min         3.07
_exptl_absorpt_coefficient_mu    42.513
_exptl_crystal_density_diffrn    5.462
_exptl_crystal_F_000             692
_refine_diff_density_max         2.989
_refine_diff_density_min         -1.819
_refine_diff_density_rms         0.409
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.232
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         220
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.232
_refine_ls_R_factor_all          0.0549
_refine_ls_R_factor_gt           0.0494
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0874P)^2^+5.9745P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1330
_refine_ls_wR_factor_ref         0.1389
_reflns_number_gt                193
_reflns_number_total             220
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic0503572Bsi20050308_041814.cif
_cod_data_source_block           tp_31c
_cod_original_cell_volume        491.43(14)
_cod_database_code               4327330